Vertical heterostructures combining different layered materials offer novel opportunities for applications and fundamental studies. Here we report a new class of heterostructures comprising a single-layer (or bilayer) graphene in close proximity to a quantum well created in GaAs and supporting a high-mobility two-dimensional electron gas. In our devices, graphene is naturally hole-doped, thereby allowing for the investigation of electron–hole interactions. We focus on the Coulomb drag transport measurements, which are sensitive to many-body effects, and find that the Coulomb drag resistivity significantly increases for temperatures <5–10 K. The low-temperature data follow a logarithmic law, therefore displaying a notable departure from the ordinary quadratic temperature dependence expected in a weakly correlated Fermi-liquid. This anomalous behaviour is consistent with the onset of strong interlayer correlations. Our heterostructures represent a new platform for the creation of coherent circuits and topologically protected quantum bits.
Solid-state dipolar quantum liquids are many-particle systems of repulsively interacting dipoles made of electron–hole (e–h) pairs, which have been studied for the past 50 years (for recent reviews, see for example, refs 1, 2). These systems display a rich and intriguing phenomenology. Particular attention has been devoted to the Bose–Einstein condensation (BEC) of e–h pairs, that is, exciton condensation, with notable results1,2. Optical signatures of BEC of excitons have been reported in optically excited exciton3,4,5 and exciton–polariton6 cold gases, where, however, non-equilibrium effects conflict, to some extent, with equilibrium thermodynamics. Spectacular implications of spontaneous coherence on transport have also been discovered in systems of permanent (interlayer) excitons7. Quantum Hall fluids in high-mobility GaAs/AlGaAs semiconductor double quantum wells display a large variety of transport anomalies8,9 due to spontaneous coherence of interlayer excitons.
There is an ongoing effort to find new systems that display spontaneous coherence and superfluidity of permanent excitons. In addition to the fundamental interest in understanding when these phenomena occur in nature, there is a practical interest in discovering many-particle systems where these types of orders occur under less extreme physical conditions, in particular in the absence of strong magnetic fields and, possibly, at non-cryogenic temperatures. Interest in interlayer excitons has been recently revitalized10,11,12 by theoretical predictions of high-temperature spontaneous coherence and superfluidity in electrically decoupled graphene layers13,14,15 and topological insulator thin films16,17,18,19. The former systems are just examples of van der Waals heterostructures20 in which different layered materials are combined to offer novel opportunities for applications21,22,23 and fundamental studies10,11,12.
In the following, we report a new class of vertical heterostructures comprising a single-layer, SLG (or bilayer, BLG) graphene carrying a fluid of massless (massive) chiral holes in close proximity to a GaAs quantum well hosting a high-mobility two-dimensional (2D) electron gas. We focus on the Coulomb drag transport measurements, which are sensitive to many-body effects. We find that the Coulomb drag resistivity significantly increases for temperatures T<5–10 K, with a notable departure from the T2 temperature dependence expected in a weakly correlated Fermi-liquid scenario24. The low-temperature data follow a logarithmic law, without the onset of saturation in the case of bilayer graphene/GaAs samples. This anomalous behaviour is consistent with the onset of strong interlayer correlations. These heterostructures may offer new routes for the exploration of a variety of e–h phenomena, including coherent circuits with minimal dissipation25,26,27 and nanodevices including analogue-to-digital converters28 and topologically protected quantum bits29.
Sample design and characterization
Our vertical heterostructures are prepared as follows: SLG and BLG flakes are produced by micromechanical exfoliation of graphite on Si/SiO2 (ref. 30). The number of layers is identified by a combination of optical microscopy31 and Raman spectroscopy32,33. The latter is also used to monitor the sample quality by measuring the D to G ratio34 and the doping level35. Selected flakes are then placed onto a GaAs-based substrate at the centre of a pre-patterned Hall bar by using a polymer-based wet transfer process22 (for details, see Supplementary Note 1). The GaAs-based substrates consist of modulation-doped GaAs/AlGaAs heterostructures hosting a 2D electron gas (2DEG) in the GaAs quantum well placed 31.5 nm below the surface. The heterostructures are grown by molecular beam epitaxy36 and consist of a n-doped GaAs cap layer, a AlGaAs barrier, a GaAs well and a thick AlGaAs barrier with a delta doping layer (see Supplementary Fig. 1). Two different samples are fabricated: sample A, with a 15-nm-thick quantum well, and sample B, with a 22-nm quantum well. Hall bars (300 μm wide and 1,500 μm long) are fabricated by ultraviolet lithography. Ni/AuGe/Ni/Au layers are then evaporated and annealed at 400 °C to form Ohmic contacts to the 2DEG, to be used for transport and the Coulomb drag measurements (see Fig. 1). The Hall bar mesas are defined by conventional wet etching in acid solution. To ensure that the current in the 2DEG flows only in the region below the graphene flakes, channels with a width comparable to the transferred graphene flakes (typically ~30 μm) are defined in the Hall bar by electron beam lithography and wet etching (Fig. 1e,f). A SLG flake is transferred onto sample A and a BLG flake onto sample B. The integrity of the SLG and BLG flakes is monitored throughout the process by Raman spectroscopy. Supplementary Fig. 2 compares the Raman spectra of the as-prepared SLG on Si/SiO2 and after transfer on GaAs. The analysis of G peak position, Pos(G), its full width at half maximum, FWHM(G), Pos(2D) and the area and intensity ratios of 2D and G peaks allow us to monitor the amount and type of doping33,35,37,38. This indicates a small p-doping for the as-prepared sample, decreasing to below 100 meV for the transferred sample33,35,37. The absence of a significant D peak both before and after transfer indicates that the samples have negligible amount of defects33,34 and that the transfer procedure does not add defects. Similarly, no increase in defects is seen for the BLG samples.
To ensure that the 2D chiral hole gas in SLG/BLG and the 2DEG in GaAs are electrically isolated, we monitor the interlayer II–VI characteristics in the T=0.25–50 K temperature range (see Supplementary Note 2), with II and VI the interlayer (‘leakage’) current and interlayer voltage, respectively, and the layers being the SLG (or BLG) and the GaAs quantum well. In SLG-based devices, a negligible interlayer current <0.2 nA is measured for VI up to −0.3 V for all values of T, leading to interlayer resistances ~1 GΩ. In the case of BLG, for T~45 K, II increases to 100 nA at VI=−0.3 V, with the interlayer resistance increasing to several MΩ. In all cases, therefore, the interlayer resistance is much larger than the largest intralayer resistance for SLG, BLG and GaAs quantum well, which is ~10 kΩ.
Magnetotransport and the Coulomb drag measurements
To search for signatures of correlations between the 2DEG in the GaAs quantum well and the 2D chiral hole fluid39 in SLG or BLG, we measure the T dependence of the Coulomb drag resistance RD. Experimentally, the Coulomb drag is routinely used as a sensitive probe of strong correlations including transitions to the superconducting state40, metal-insulator transitions41 and Luttinger liquid correlations42 in quantum wires, and exciton condensation in quantum Hall bilayers9. In a Coulomb drag experiment24,43,44, a current source is connected to one of the two layers (the active or drive layer). The other layer (the passive layer) is connected to an external voltmeter so that the layer can be assumed to be an open circuit (no current can flow in it). The drive current Idrive drags carriers in the passive layer, which accumulate at the ends of the layer, building up an electric field. The voltage drop Vdrag related to this field is then measured. The quantity RD is defined as the ratio Vdrag/Idrive and is determined by the rate at which momentum is transferred between quasiparticles in the two layers24. Before the Coulomb drag experiments, we performed magnetotransport measurements at 4 K, as for Fig. 2a,b. In our set-up, the 2DEG is induced in the quantum well by shining light from an infrared diode. In the SLG/2DEG device, we find a 2DEG with density n=1.2 × 1011 cm−2 from low-field (below 1 T) classical Hall effect and a mobility μe=13,000 cm2 V−1 s−1 at 4 K. At T=45 K, the density decreases to 4.0 × 1010 cm−2 and μe=8,700 cm2 V−1 s−1. Figure 2a) shows the quantum Hall effect in the 2DEG. The quantum Hall plateaus at h/(2e2) and h/(4e2) (blue trace) correspond to the first two spin degenerate Landau levels45. In correspondence of the plateaus, minima are found45 in the longitudinal resistance Rxx (red trace).
The 2D chiral hole fluids in SLG and BLG have their highest mobility when the 2DEG is not induced. This is shown in Fig. 2b for the SLG-based device (see also Supplementary Note 3). Figure 2a,b indicates that the sign of the Hall resistance Rxy in SLG is opposite to the 2DEG, thereby demonstrating that SLG is p-doped. At 4 K, the hole density is p=9.9 × 1011 cm−2 and μh=4,100 cm2 V−1 s−1. At 45 K, the corresponding values are p=6.7 × 1011 cm−2 and μh=2,400 cm2 V−1 s−1. Low-T magnetotransport in SLG (Fig. 2b) reveals quantum Hall plateaus at h/(2e2) and h/(6e2), corresponding to the massless Dirac fermions with spin and valley degeneracy39. On the contrary, when the 2DEG is optically induced, the hole density in SLG at 4 K is p=6.7 × 1011 cm−2 and μh=2,100 cm2 V−1 s−1, thereby weakening the manifestations of the quantum Hall effect (see Supplementary Fig. 3). The degradation of the SLG transport properties in the presence of the 2DEG could be linked to the creation of ionized Si donors within the n-doped GaAs cap layer, acting as positively charged scatterers46.
We now focus on the Coulomb drag experiments. These are performed in the configuration sketched in Fig. 1a,b and in a 3He cryostat with a 240 mK–50 K range. Ten Vdrag−Idrive curves in a d.c. configuration are acquired for each T and then averaged. We first address the SLG/2DEG case. Figure 2c reports a representative set of averaged drag voltage data taken in the 2DEG at T=42.5 K. In this configuration, the SLG gating effect and consequent carrier depletion in the 2DEG are avoided by applying a positive current, from 0 to +2 μA in the SLG channel. Figure 2c) shows that, at this representative T, the drag voltage is linear with the drive current, thereby allowing the extraction of RD from the slope of a linear fit. Figure 2d shows the plots of RD for 30 K≤T≤50 K, with the 2DEG used as the drive (black points) or passive (red points) layer. It also reports calculations of the temperature dependence of RD in a hybrid Dirac/Schrödinger SLG/2DEG double layer within a Boltzmann-transport theory, which is justified in the Fermi-liquid regime47,48. This is done by generalizing the theory of ref. 47 to include effects due to the finite width of the GaAs quantum well (see Supplementary Note 4). This shows that the experimental results in this temperature range are consistent with the canonical Fermi-liquid prediction24,43,44,45,46,47,48,49,50, that is, RD∝T2 (see also Fig. 3a), as constrained by the available phase-space of the initial and final states involved in the scattering process. The magnitude of the measured effect, however, is smaller than predicted by theory. Discrepancies of similar magnitude have been previously reported for the Coulomb drag measurements between two SLGs encapsulated in hexagonal boron nitride11. Figure 2d demonstrates that the Onsager reciprocity relations51, which in our case require that the resistance measured by interchanging drive and passive layers should not change, are satisfied in the 30 K≤T≤40 K range. A violation of reciprocity occurs for T>40 K. We ascribe this to the effect of the interlayer current II, leading to an additional contribution sensitive to the exchange of active and passive layers (see Supplementary Note 2 and Supplementary Fig. 4). Consistent with this interpretation, we observe larger violations of Onsager reciprocity in the BLG/GaAs sample, where II is three orders of magnitude larger than SLG/GaAs at T=45 K (see Supplementary Fig. 5). We now discuss the behaviour of RD in the low-temperature regime. We follow ref. 11 and use the lowest quality layer, in our case SLG, as the drive layer and measure the drag voltage in the 2DEG. In the reversed configuration, the drag voltage measured in SLG shows fluctuations11,12 as a function of the drive current, which hamper the extraction of RD, see Supplementary Note 5). RD measured in the 2DEG reveals an anomalous behaviour below 10 K. Figure 3 indicates that RD deviates from the ordinary T2 dependence, as shown by a large upturn for T lower than an ‘upturn’ temperature Tu~5 K. The enhancement of RD at low T is a very strong effect: the drag signal increases by more than one order of magnitude by decreasing T below Tu, where RD is vanishingly small, in agreement with the Fermi-liquid predictions (see Supplementary Note 4), down to T=240 mK.
Figure 3b is a zoom of the drag enhancement data in the low-T range together with a fit (solid line) of the type:
where R0 and A are two fitting parameters and Tc indicates the mean-field critical temperature of a low-T phase transition at which the drag resistance would display a weak singularity. This fitting procedure cannot predict Tc: for example, fixing Tc=10 mK, the best-fit yields A=(0.416±0.015) Ω and R0=(2.66±0.08) Ω. We can well fit the experimental data by choosing any value of Tc, as long as this is substantially lower than the lowest investigated temperature, that is, T=240 mK. As it is clear from the functional form of the fitting function in equation (1), in this regime a change can be reabsorbed into a change of the background resistance . Despite this caveat, we note that our fitting procedure is in excellent agreement with the data for Tc in the range 10–100 mK.
We note, however, that the data point at the lowest measured T=240 mK deviates from the logarithmic trend, possibly pointing to the onset of saturation. To further investigate this, we explore a second device comprising of a hole-doped exfoliated BLG deposited on the surface of a GaAs quantum heterostructure. The hole density in BLG is p=1.4 × 1012 cm−2 from the low-field (below 1 T) classical Hall effect and the mobility is 670 cm2 V−1 s−1 at 4 K. The 2DEG has an electron density n=2 × 1011 cm−2 and a mobility 86,000 cm2 V−1 s−1 at 4 K. Contrary to the SLG/2DEG case, in the BLG/2DEG device, both electron and hole fluids have parabolic energy–momentum dispersions (Fig. 4b,c). A lower kinetic energy in BLG (vanishing like k2 (ref. 39) rather than like k for small values of momentum ℏk) compared with SLG is expected to enhance the relative importance of Coulomb interactions52. It is therefore interesting to evaluate whether this enhancement manifests in the low-temperature drag resistance. To probe this, we measure the evolution of RD as a function of T using BLG as the drive layer (See Supplementary Figs. 6 and 7). Figure 4 again shows a significant departure from the Fermi-liquid T2 dependence. Consistent with the expected larger impact of interactions52,53, we get Tu~10 K, that is, twice the SLG/2DEG case, while the best-fit of RD data based on equation (1) yields Tc=190 mK (to be compared with Tc=10–100 mK in the SLG/2DEG). The observed drag resistance remains two–three orders of magnitude smaller than the layer resistance. However, if we follow the logarithmic increase of the drag signal as T approaches Tc, the drag resistance can reach arbitrarily large values, of the order of 102–103 Ω (that is, comparable to the isolated-layer resistance).
The observed upturn of the drag resistance as a function of T is puzzling and so is the fact that the experimental data in the upturn regime are well fitted by a logarithmic function, rather than an exponential or a power law. We now elaborate on possible explanations of this phenomenology. Ref. 5454 predicted a finite value of the drag resistivity at T=0 as a consequence of higher-order effects in perturbation theory (third order in the interlayer interaction). The predicted value of interaction-induced drag, however, is far too small (≈10−5 Ω per square) to explain our upturn. Mesoscopic effects can lead both to positive and negative fluctuations of the low-temperature drag resistivity as a function of the electron density55. In our experiments, however, the upturn is fully reproducible for different devices (SLG/GaAs and BLG/GaAs) and cool downs (yielding slightly different densities). We therefore exclude that this effect is responsible for the logarithmic increase. Finally, the disorder effects in the diffusive regime49,50 do lead to a logarithmic enhancement of the drag signal of the form RD(T)∝−T2 log(T) for T→0, which is therefore a correction to the Fermi-liquid behaviour and not an upturn.
The logarithmic enhancement of RD described by equation (1) was theoretically predicted in refs 17, 18 on the basis of a Boltzmann-transport theory for e–h double layers, where the scattering amplitude is evaluated in a ladder approximation56. Similar results were obtained on the basis of a Kubo-formula approach57. Within these frameworks, the enhancement is attributed to e–h pairing fluctuations extending above Tc for a phase transition into an exciton condensed phase1,17,18,57,58. If this scenario is correct, Fig. 3b indicates that the T range above Tc, in which fluctuations are responsible for deviations from the Fermi-liquid T2 dependence, is very large. This can be ascribed to the quasi-2D nature of our SLG/2DEG heterostructure and shares similarities with other 2D systems where fluctuations play an important role, such as cuprate superconductors (see, for example, ref. 59) and ultracold Fermi gases60.
The mismatch in the Fermi wave numbers , which is ~25% in the SLG/2DEG and ΔkF~30% in the BLG/2DEG case, raises concern on the validity of the exciton-condensate scenario. (Here and are the Fermi wave numbers in the layers with n- and p-doping, respectively.) Indeed, such a mismatch is expected61 to weaken the robustness of the exciton-condensate phase in which the condensed e–h pairs have zero total momentum ℏK. However, preliminary calculations including screening in the condensed phase62,63,64 indicate that the K=0 exciton-condensate state persists even in the presence of these values of ΔkF, with Tc scales comparable to those reported here. On the other hand, a mismatch in the Fermi wave numbers of the two fluids may favour Fulde–Ferrell–Larkin–Ovchinnikov65 or Sarma66 phases. These are however rather fragile in dimensionality d>1, although evidence of a Fulde–Ferrell–Larkin–Ovchinnikov phase was reported, for example, in the layered heavy-fermion superconductor CeCoIn5 (ref. 67).
We stress that a perfect matching condition would be essential for the exciton-condensate scenario if the system was in the BCS weak-coupling regime, where a small density imbalance leads to a chemical potential difference greater than the pairing gap, and this would indeed destroy superfluidity. However, it was shown theoretically that e–h superfluidity can only appear at experimentally reachable temperatures when the system is already in the so-called BCS–BEC crossover64. In this regime, superfluidity is robust against density imbalance, and there is strong evidence from both theory and experiment61,68,69 that it is not killed by the Fermi surface mismatches up to 50%.
Finally, we recall that upturns of the Coulomb drag resistivity were reported in e–h doped GaAs/AlGaAs coupled quantum wells70,71,72. However, the combination of 2D electron and hole gases in the same GaAs material required a large nanofabrication effort, and the reported magnitude of the drag anomalies was smaller than in our hybrid heterostructures.
Our observations establish a new class of vertical heterostructure devices with a potentially large flexibility in the design of band dispersions, doping and e–h coupling, where excitonic phenomena are accessible.
How to cite this article: Gamucci, A. et al. Anomalous low-temperature Coulomb drag in graphene-GaAs heterostructures. Nat. Commun. 5:5824 doi: 10.1038/ncomms6824 (2014).
Snoke, D. Spontaneous Bose coherence of excitons and polaritons. Science 298, 1368–1372 (2002).
Rontani, M. & Sham, L. J. inNovel Superfluids Vol. 2, International Series of Monographs on Physics no. 157 (eds Bennemann K. H., Ketterson J. B. Oxford Univ. Press (2013).
Butov, L. V. Cold exciton gases in coupled quantum well structures. J. Phys.: Condens. Matter 19, 295202 (2007).
High, A. A. et al. Spontaneous coherence in a cold exciton gas. Nature 483, 584–588 (2012).
Alloing, M. et al. Evidence for a Bose-Einstein condensate of excitons. Europhys. Lett. 107, 10012 (2014).
Kasprzak, J. et al. Bose-Einstein condensation of exciton polaritons. Nature 443, 409–414 (2006).
Lozovik, Y. E. & Yudson, V. I. Feasibility of superfluidity of paired spatially separated electrons and holes; a new superconductivity mechanism. Pis'ma Zh. Eksp. Teor. Fiz. 22, 556–559 (1975).
Eisenstein, J. P. & MacDonald, A. H. Bose-Einstein condensation of excitons in bilayer electron systems. Nature 432, 691–694 (2004).
Nandi, D., Finck, A. D. K., Eisenstein, J. P., Pfeiffer, L. N. & West, K. W. Exciton condensation and perfect Coulomb drag. Nature 488, 481–484 (2012).
Kim, S. et al. Coulomb drag of massless fermions in graphene. Phys. Rev. B 83, 161401(R) (2011).
Gorbachev, R. V. et al. Strong Coulomb drag and broken symmetry in double-layer graphene. Nat. Phys. 8, 896–901 (2012).
Kim, S. & Tutuc, E. Coulomb drag and magnetotransport in graphene double layers. Solid State Commun. 152, 1283–1288 (2012).
Min, H., Bistritzer, R., Su, J.-J. & MacDonald, A. H. Room-temperature superfluidity in graphene bilayers. Phys. Rev. B 78, 121401(R) (2008).
Zhang, C.-H. & Joglekar, Y. N. Excitonic condensation of massless fermions in graphene bilayers. Phys. Rev. B 77, 233405 (2008).
Lozovik, Y. E. & Sokolik, A. A. Electron-hole pair condensation in graphene bilayer. JETP Lett. 87, 55 (2008).
Seradjeh, B., Moore, J. E. & Franz, M. Exciton condensation and charge fractionalization in a topological insulator film. Phys. Rev. Lett. 103, 066402 (2009).
Mink, M. P., Stoof, H. T. C., Duine, R. A., Polini, M. & Vignale, G. Probing the topological exciton condensate via Coulomb drag. Phys. Rev. Lett. 108, 186402 (2012).
Mink, M. P., Stoof, H. T. C., Duine, R. A., Polini, M. & Vignale, G. Unified Boltzmann transport theory for the drag resistivity close to an interlayer-interaction-driven second-order phase transition. Phys. Rev. B 88, 235311 (2013).
Efimkin, D. K., Lozovik, Y. u. E. & Sokolik, A. A. Electron-hole pairing in a topological insulator thin film. Phys. Rev. B 86, 115436 (2012).
Geim, A. K. & Grigorieva, I. V. Van der Waals heterostructures. Nature 499, 419–425 (2013).
Novoselov, K. S. & Castro Neto, A. H. Two-dimensional crystals-based heterostructures: materials with tailored properties. Phys. Scr. T146, 014006 (2012).
Bonaccorso, F. et al. Production and processing of graphene and 2D crystals. Mater. Today 15, 564–589 (2012).
Britnell, L. et al. Field-effect tunneling transistor based on vertical graphene heterostructures. Science 335, 947–950 (2012).
Rojo, A. G. Electron-drag effects in coupled electron systems. J. Phys.: Condens. Matter 11, R31 (1999).
High, A. A., Novitskaya, E. E., Butov, L. V. & Gossard, A. C. Control of exciton fluxes in an excitonic integrated circuit. Science 321, 229–231 (2008).
Kuznetsova, Y. Y. et al. All-optical excitonic transistor. Optics Lett. 35, 1587–1589 (2010).
Ballarini, D. et al. All-optical polariton transistor. Nat. Commun. 4, 1778 (2013).
Dolcini, F. et al. Blockade and counterflow supercurrent in exciton-condensate Josephson junctions. Phys. Rev. Lett. 104, 027004 (2010).
Peotta, S. et al. Josephson current in a four-terminal superconductor/exciton-condensate/superconductor system. Phys. Rev. B 84, 184528 (2011).
Novoselov, K. S. et al. Two-dimensional atomic crystals. Proc. Natl Acad. Sci. USA 102, 10451–10453 (2005).
Casiraghi, C. et al. Rayleigh imaging of graphene and graphene layers. Nano Lett. 7, 2711–2717 (2007).
Ferrari, A. C. et al. Raman spectrum of graphene and graphene layers. Phys. Rev. Lett. 97, 187401 (2006).
Ferrari, A. C. & Basko, D. M. Raman spectroscopy as a versatile tool for studying the properties of graphene. Nat. Nanotechnol. 8, 235–246 (2013).
Cancado, L. G. et al. Quantifying defects in graphene via Raman spectroscopy at different excitation energies. Nano Lett. 11, 3190–3196 (2011).
Das, A. et al. Monitoring dopants by Raman scattering in an electrochemically top-gated graphene transistor. Nat. Nanotechnol. 3, 210–215 (2008).
Pfeiffer, L. N. & West, K. W. The role of MBE in recent quantum Hall effect physics discoveries. Physica E 20, 57–64 (2003).
Basko, D. M., Piscanec, S. & Ferrari, A. C. Electron-electron interactions and doping dependence of the two-phonon Raman intensity in graphene. Phys. Rev. B 80, 165413 (2009).
Bruna, M. et al. Doping dependence of the Raman Spectrum of defected graphene. ACS Nano 8, 7432–7441 (2014).
Geim, A. K. & Novoselov, K. S. The rise of graphene. Nat. Mater. 6, 183–191 (2007).
Giordano, N. & Monnier, J. D. Cross-talk effects in superconductor-insulator-normal-metal trilayers. Phys. Rev. B 50, 9363–9368 (1994).
Pillarisetty, R. et al. Coulomb drag near the metal-insulator transition in two dimensions. Phys. Rev. B 71, 115307 (2005).
Laroche, D., Gervais, G., Lilly, M. P. & Reno, J. L. 1D-1D Coulomb drag signature of a Luttinger liquid. Science 343, 631–634 (2014).
Gramila, T. J., Eisenstein, J. P., MacDonald, A. H., Pfeiffer, L. N. & West, K. W. Mutual friction between parallel two-dimensional electron systems. Phys. Rev. Lett. 66, 1216–1219 (1991).
Sivan, U., Solomon, P. M. & Shtrikman, H. Coupled electron-hole transport. Phys. Rev. Lett. 68, 1196–1199 (1992).
Prange, R. E. & Girvin, S. M. The Quantum Hall Effect Springer-Verlag (1990).
Das Sarma, S., Adam, S., Hwang, E. H. & Rossi, E. Electronic transport in two-dimensional graphene. Rev. Mod. Phys. 83, 407–470 (2011).
Principi, A., Carrega, M., Asgari, R., Pellegrini, V. & Polini, M. Plasmons and Coulomb drag in Dirac/Schrödinger hybrid electron systems. Phys. Rev. B 86, 085421 (2012).
Carrega, M., Tudorovskiy, T., Principi, A., Katsnelson, M. I. & Polini, M. Theory of Coulomb drag for massless Dirac fermions. New J. Phys. 14, 063033 (2012).
Zheng, L. & MacDonald, A. H. Coulomb drag between disordered two-dimensional electron-gas layers. Phys. Rev. B 48, 8203–8209 (1993).
Kamenev, A. & Oreg, Y. Coulomb drag in normal metals and superconductors: diagrammatic approach. Phys. Rev. B 52, 7516–7527 (1995).
Casimir, H. B. G. On Onsager’s principle of microscopic reversibility. Rev. Mod. Phys. 17, 343 (1945).
Giuliani, G. F. & Vignale, G. Quantum Theory of the Electron Liquid Cambridge Univ. Press (2005).
Perali, A., Neilson, D. & Hamilton, A. R. High-temperature superfluidity in double-bilayer graphene. Phys. Rev. Lett. 110, 146803 (2013).
Levchenko, A. & Kamenev, A. Coulomb drag at zero temperature. Phys. Rev. Lett. 100, 026805 (2008).
Price, A. S., Savchenko, A. K., Narozhny, B. N., Allison, G. & Ritchie, D. A. Giant fluctuations of Coulomb drag in a bilayer system. Science 316, 99–102 (2007).
Larkin, A. & Varlamov, A. Theory of Fluctuations in Superconductors Clarendon Press (2004).
Hu, B. Y.-K. Prospecting for the superfluid transition in electron-hole coupled quantum wells using Coulomb drag. Phys. Rev. Lett. 85, 820–823 (2000).
Rist, S., Varlamov, A. A., MacDonald, A. H., Fazio, R. & Polini, M. Photoemission spectra of massless Dirac fermions on the verge of exciton condensation. Phys. Rev. B 87, 075418 (2013).
Zhang, W. et al. Signatures of superconductivity and pseudogap formation in nonequilibrium nodal quasiparticles revealed by ultrafast angle-resolved photoemission. Phys. Rev. B 88, 245132 (2013).
Feld, M., Fröhlich, B., Vogt, E., Koschorreck, M. & Köhl, M. Observation of a pairing pseudogap in a two-dimensional Fermi gas. Nature 480, 75–78 (2011).
Pieri, P., Neilson, D. & Strinati, G. C. Effects of density imbalance on the BCS-BEC crossover in semiconductor electron-hole bilayers. Phys. Rev. B 75, 113301 (2007).
Sodemann, I., Pesin, D. A. & MacDonald, A. H. Interaction-enhanced coherence between two-dimensional Dirac layers. Phys. Rev. B 85, 195136 (2012).
Lozovik, Y. u. E., Ogarkov, S. L. & Sokolik, A. A. Condensation of electron-hole pairs in a two-layer graphene system: correlation effects. Phys. Rev. B 86, 045429 (2012).
Neilson, D., Perali, A. & Hamilton, A. R. Excitonic superfluidity and screening in electron-hole bilayer systems. Phys. Rev. B 89, 060502(R) (2014).
Casalbuoni, R. & Nardulli, G. Inhomogeneous superconductivity in condensed matter and QCD. Rev. Mod. Phys. 76, 263–320 (2004).
Subas, A. L., Pieri, P., Senatore, G. & Tanatar, B. Stability of Sarma phases in density imbalanced electron-hole bilayer systems. Phys. Rev. B 81, 075436 (2010).
Bianchi, A., Movshovich, R., Capan, C., Pagliuso, P. G. & Sarrao, J. L. Possible Fulde-Ferrell-Larkin-Ovchinnikov superconducting state in CeCoIn5 . Phys. Rev. Lett. 91, 187004 (2003).
Shin, Y.-I., Schunck, C. H., Schirotzek, A. & Ketterle, W. Phase diagram of a two-component Fermi gas with resonant interactions. Nature 451, 689–693 (2008).
Lobo, C., Recati, A., Giorgini, S. & Stringari, S. Normal state of a polarized Fermi gas at unitarity. Phys. Rev. Lett. 97, 200403 (2006).
Croxall, A. F. et al. Anomalous Coulomb drag in electron-hole bilayers. Phys. Rev. Lett. 101, 246801 (2008).
Seamons, J. A., Morath, C. P., Reno, J. L. & Lilly, M. P. Coulomb drag in the exciton regime in electron-hole bilayers. Phys. Rev. Lett. 102, 026804 (2009).
Morath, C. P., Seamons, J. A., Reno, J. L. & Lilly, M. P. Density imbalance effect on the Coulomb drag upturn in an undoped electron-hole bilayer. Phys. Rev. B 79, 041305(R) (2009).
We thank R. Duine, R. Fazio, A. Hamilton, M. Katsnelson, A. MacDonald, D. Neilson, K. Novoselov, A. Perali, A. Pinczuk and G. Vignale for very useful discussions. We acknowledge funding from the EU Graphene Flagship (contract no. CNECT-ICT-604391), the EC ITN project ‘INDEX’ Grant No. FP7-2011-289968, the Italian Ministry of Education, University and Research (MIUR) through the programs ‘FIRB—Futuro in Ricerca 2010’ Grant No. RBFR10M5BT (‘PLASMOGRAPH’) and ‘Progetti Premiali 2012’ (Project ‘ABNANOTECH’), ERC grants NANOPOTS, Hetero2D, a Royal Society Wolfson Research Merit Award, EU projects GENIUS, CARERAMM, RODIN, EPSRC grants EP/K01711X/1, EP/K017144/1 and EP/L016087/1.
The authors declare no competing financial interests.
About this article
Cite this article
Gamucci, A., Spirito, D., Carrega, M. et al. Anomalous low-temperature Coulomb drag in graphene-GaAs heterostructures. Nat Commun 5, 5824 (2014). https://doi.org/10.1038/ncomms6824
This article is cited by
Nature Physics (2023)
Applied Physics A (2021)
Synthesis of lateral heterostructure of 2D materials for optoelectronic devices: challenges and opportunities
Emergent Materials (2021)
Photon-generated carrier transfer process from graphene to quantum dots: optical evidences and ultrafast photonics applications
npj 2D Materials and Applications (2020)
Communications Physics (2018)